Main Article Content
An adequate mixing time in concrete casting allows to achieve a homogeneous mass and improve compressive strength and durability. However, the lack of standards for cast-in-place concrete causes that the builders use different mixing times according to the locality usages and customs, which results in a high variability of the expected quality. In this paper, fresh and hardened cast-in-place concrete was evaluated. Seven samples were tested with different mixing time using portable rotary drum mixer. The used materials were ordinary portland cement, water and high absorption aggregates, fine and coarse, coming from a limestone crushing process. The results of the research showed that the mixing time and environmental temperature had no apparent influence on the slump of the mixtures, and trapped air and compressive strength increased slightly with increasing mixing time. Finally, it was found that the recommended mixing time, with rotation speed of 28 RPM, is 2.5 minutes, which differs from the common practice in the study area.
NMX C-159-ONNCCE-1999. Industria de la Construcción-Concreto-Elaboración y Curado de Especímenes en el laboratorio. México: Organismo Nacional de Normalización y Certificación de la Construcción y Edificación, S. C; 1999.
ASTM C 94-13. Standard Specification for Ready Mixed Concrete. West Conshohocken, (PA): American Society for Testing and Materials; 2013.
ACI 304 R-00. Guide for Measuring, Mixing, Transporting, and Placing Concrete. Farmington Hills (MI): American Concrete Institute; 2000.
NMX C-403-ONNCCE-1999. Industria de la Construcción-Concreto Hidráulico para Uso Estructural. México: Organismo Nacional de Normalización y Certificación de la Construcción y Edificación, S. C; 1999.
ACI Committee 318. Building Code Requirements for Structural Concrete and Commentary. Farmington Hills (MI): American Concrete Institute; 2014.
Neville AM, Brooks JJ. Tecnología del concreto. 1st ed. México: Trillas; 2010.
Charonnat Y, Beitzel H. Efficiency of concrete mixers towards qualifications of mixers. Mater Struct, RILEM. 1997; (Supplement):32-28. Available:https://doi.org/10.1007/BF02539273
Trejo D, Chen J. Effects of extended discharge time and revolution counts for ready-mixed concrete. Research Project SPR. Final Report. Oregon State University; 2014.
Instituto Nacional de Estadística y Geografía. Censo de Población y Vivienda 2010; 2013.
ASTM Book of Standards, Construction: Concrete and Aggregates, American Society for Testing and Materials, West Conshohocken, PA, USA; 2010.
Trejo-Arroyo DL, Acosta KE, Cruz JC, Valenzuela-Muñiz AM, Vega-Azamar RE, Jiménez LF. Inﬂuence of ZrO2 nano-particles on the micro structural develop-ment of cement mortars with limestone aggregates. Appl. Sci. 2019;598(9):12.
ASTM C 33-08; Standard Specification for Concrete Aggregates, American Society for Testing and Materials, West Conshohocken, PA, USA; 2008.
ACI 211.1; Standard Practice for Selecting Proportions for Normal, Heavyweight and Mass Concrete, American Concrete Institute, Farmington Hills, MI, USA; 1998.
González-Diaz E, Jaizme-Vega E, Jubera-Pérez J. Assessment of the influence of the effective water-cement ratio on the workability and strength of a commercial concrete used for the construction of concrete caissons. Rev. Constr. 2018; 32(2):239-231.
Kirka Ö, Turanli L, Erdoǧan T. Effects of retempering on consistency and compres-sive strength of concrete subjected to prolonged mixing. Cem. Concr. Res. 2002; 32(3):445-441.
Trejo D, Chen J. Influence of mixing time on fresh and hardened concrete characteristics. ACI Mater. J. 2015;112(6): 754-745.
Montgomery DC. Diseño y análisis de experimentos, Limusa Wiley: México, 2011.